UNIVERSITI TEKNIKAL MALAYSIA MELAKA (UTeM)
EFFECT OF DIFFERENT COATING LAYER OF ALKALI NIOBATE (KNN) THIN FILM THROUGH SOL-GEL TECHNIQUE
This report is summited with requirement of the Universiti Teknikal Malaysia Melaka (UTeM) for the Bachelor Degree of Manufacturing Engineering
(Engineering Materials) (Hons.)
MOHD SYARIZAL BIN ANUAR B051110231
UNIVERSITI TEKNIKAL MALAYSIA MELAKA
BORANG PENGESAHAN STATUS LAPORAN PROJEK SARJANA MUDA
TAJUK: Investigation of mechanical and morphological properties of spent bleach earth (SBE) reinforced glass waste composite
SESI PENGAJIAN: 2014/15 Semester 2
Saya MOHD SYARIZAL BIN ANUAR
mengaku membenarkan Laporan PSM ini disimpan di Perpustakaan Universiti Teknikal Malaysia Melaka (UTeM) dengan syarat-syarat kegunaan seperti berikut:
1. Laporan PSM adalah hak milik Universiti Teknikal Malaysia Melaka dan penulis. 2. Perpustakaan Universiti Teknikal Malaysia Melaka dibenarkan membuat salinan
untuk tujuan pengajian sahaja dengan izin penulis.
I hereby, declared this report entitled ‘Effect of different coating layer of alkali niobate (KNN) thin film through sol-gel technique’ is the results of my own research except as cited in references.
Signature : ………
This report is submitted to the Faculty of Manufacturing Engineering of UTeM as a partial fulfillment to the requirements for the degree of Bachelor of Manufacturing Engineering (Engineering Materials) (Hons.). The member of the supervisory is as follow:
To my parents and family member for their continuous support through my study.
To my supervisor and postgraduate student for their advice and guidance in completing this research.
First of all, I would like to express my gratitude to Allah The Almighty for giving me the health to complete my Final Year Project. I would like to thank both my parents for their continuous support and help in order to complete my research. I would also like to thank my supervisor, PM Dr Mohd Warikh Bin Abd Rashid who willing to spare his time in guiding and share his experience for me to complete this research. Without his help, I would not be able to complete this research on time.
I would also like to thank all my friends who have support and willing to help me whenever I faced any problem in completing the research and the report.
TABLE OF CONTENT
Table of Content ⅲ
List of Table ⅶ
List of Figures ⅷ
CHAPTER 1: INTRODUCTION 1
1.1 Background 1
1.2 Problem Statement 2
1.3 Objectives 4
1.4 Scope 4
CHAPTER 2: LITERATURE REVIEW 5
2.1 Introduction 5
2.2 Piezoelectric 5
2.2.1 Piezoelectric Effect 6
126.96.36.199 Permittivity 7
2.7.2 Thin Film Application 10
2.6 Deposition of Thin Film 11
2.6.1 Physical Deposition 11
188.8.131.52 Sputtering 11
184.108.40.206 Thermal Evaporator 12
2.6.2 Chemical Deposition 13
220.127.116.11 Atomic Layer Deposition (ALD) 13
2.8 Characterization of Material 17
2.8.1 X-ray diffraction (XRD) 17
2.9 Morphology analysis 18
2.9.1 Microstructure Analysis 18
CHAPTER 3: METHODOLOGY 19
3.1 Introduction 19
3.2 Flow Chart of Experiment Procedure 20
3.3 Experimental Procedure 21
3.3.1 Raw material 21
3.4 Sample preparation 21
3.4.1 Sol-gel 21
3.4.1 Concentrated Sol 22
3.5 Substrate preparation 22
3.5.1 Substrate cutting 22
3.5.2 Wet chemical removal process 22
3.6 Spin Coating 23
3.7 Pyrolysis 23
3.8 Annealing 23
3.9 Scanning Electron Microscopic 24
CHAPTER 4: RESULT AND DISCUSSION 25
4.1 Introduction 25
4.2 The solution 25
4.3 X-ray diffraction (XRD) 26
4.4 Raman Spectroscopy 27
4.5 Morphological Analysis 31
4.5.1 Scanning electron microscopy 31
CHAPTER 5: CONCLUSION AND RECOMMENDATION 34
5.1 Conclusion 34
5.2 Recommendation 35
LIST OF TABLES
Table Title Page
3.1 Weight percentage in sol-gel preparation 21
LIST OF FIGURES
Figure Title Page
2.1 Sputter deposition mechanism 12
2.2 Mechanism of spin coating 14
2.3 SIO substrate 16
3.1 Flowchart of sol-gel method preparation 20
3.2 Spin coating machine 23
4.1 XRD pattern of various coting layer 26
4.2 Raman pattern of various coating layer 28
4.3 Raman peak at range of (100-1100 cm-1) wavelength 30
LIST OF ABBREVIATIONS, SYMBOLS AND
°C - degree celsius
µm - micrometre
ALD - atomic layer deposition
CH3COCH2CH2OH - acetylacetone
CH3COOK - potassium acetate
CH3COONA - sodium acetate
CH3OCH2CH2OH - 2-metoxyethanol
CVD - chemical vapour deposition
FWHM - full width half maximum
g - Gram
g/mol - gram per mol
GaAS - gallium arsenide
IC - integrated circuit
InP - indium phosphide
KNN - potassium sodium niobate
min - minute
nm - nanometre
Pt - platinum
PVD - physical vapour deposition
PZT - lead zirconate titanate
RoHS - restriction of hazardous substance
rpm - rotation per minutes
SEM - scanning electron microscope
Si - silica
SOI - silicon on insulator
TC - curie temperature
TEM - tunnelling electron microscope
Ti - titanium
WEEE - waste electrical and electronic equipment
XRD - x-ray diffraction
Rapid development in electronic industry nowadays has given a huge impact on the studies of the piezoelectric materials. The impact effected by this the demand of new material with better properties is always sought to fulfil the industry need to producing a better feature with green technology to the user. Materials like ceramics have been greatly improvised with research and development of the ceramics into a better generation of fine ceramic or also known as advance ceramic.
Advance ceramics can be made to have a wide variety of unique properties characteristic through variations in raw material, synthesizing method and processing. These unique properties can be obtained by altering the raw materials selection such as zirconia, alumina, silicon carbide and aluminium nitrate. As results, the properties of each advance ceramic material can be uniquely formulated for a specific properties, behaviour and functional according to various desired application.
One of advance ceramic that is fabricate for this purposes is piezoelectric material based on (K,Na)NbO3 due to its moderate dielectric constant and optimum
piezoelectric response as well as its friendly properties of lead-free materials. KNN has been a priority of thin film fabrication to replacing widely used lead zirconate titanate or PZT due to the facts that this ceramics contain about 60% lead, and therefore represent a possible ecological hazard, Malic et al., (2005). The switch idea of PZT to KNN is supported by the law that enforced in 2006, that the Waste Electrical and Electronic Equipment (WEEE) and restriction of the use of certain Hazardous Substances in electrical and electronic equipment (RoHS), with purpose of protecting health as well as environment by exclusion of hazardous substances in electronic devices, Li et al., (2012).
Active research was never stop to seek the best outcome possible out of advance ceramics which leads to idea of properties enhancement and manipulate of KNN structure by varies the deposition layer of KNN on Si substrate.
1.2 Problem statement
In past years, potassium sodium niobate (KNN) has been actively researched. As the only known lead free system compared to commonly use lead zirconate titanate (PZT), according to Wang, (2002) large amount of lead contained in PZT materials has drawn much attention due to environmental concern as well as regulation against hazardous substances. KNN has become the best option for replacing PZT in electrical devices, including in thin film application.
The increment of KNN coating layer was effectively proved to enhance the insulating and ferroelectric properties because of the reduced oxygen vacancies Yao, (2005). The thin films were reported to have relatively low Curie temperature, high-fatigue resistance, low-processing temperature and large remnant polarization. Watanabe, (2002) explained that the role of alkaline substituting volatile Bi-site is to suppress the A-site vacancies accompanied with oxygen vacancies which act as space charge is varies as different coating layer.
Therefore, some researchers suggested the possibility for the thin film to reduce the processing temperature and leakage current density and improve ferroelectric properties. Noguchi et al., (2002) investigate that the effect of concentration and distribution of defects controlled by quenching and doping of high-valence electron vacancies on ferroelectric properties.
The deposition of thin film technique fall into two categories which is chemical deposition and physical deposition. However, the physical deposition technique is preferred in advance thin film industry. Physical deposition technique uses mechanical, electromechanical to produce a thin film of solid. One of the techniques in physical deposition is sputtering, which relies on plasma to knock material from a ‘target’ a few atoms at a time. Sputtering is a fast technique and also provides a good thickness control of a thin film (micrometre) in thickness.
The objectives of this project are:
i. To fabricate multiple layers of KNN thin film via sol-gel method
ii. To analyze properties enhancement of KNN thin film on physical, electrical and morphological properties
The scope of this research is to analyze the crystal structure, crystal plane, polarization, dielectric and morphology of pure potassium sodium niobate (KNN) in thin film. Multiple layers of KNN will be deposited onto silicon (Si) substrate. The sample will be prepared for 5 different layers and analyzed later on.
The research is start with mixture of raw material Potassium acetate (CH3COOK),
sodium acetate (CH3COONa) and niobium pentaethoxide (Nb(OCH2CH3)5 with
2-metoxyethanol (CH3OCH2CH2OH) and acetylacetone (CH3COCH2CH2OH) as
solvent and chelating agent, using Sol-gel technique. Sol solution and Si substrate is then sputtered using spin coating machine before calcined and annealed.
The raw material preparation and substrate preparation will be fabricate and processed in parallels and both will be combined in spin coating process later on. The sol precursor of raw material via sol-gel technique will be spin coated onto SOI substrate.
This chapter is describing about the basic fundamental of piezoelectric material mainly on potassium sodium niobate (KNN) which is focused on thin film. This chapter also give brief description of the fundamental processing method of thin film piezoelectric. The characteristic of pure KNN will also be elaborated in this chapter.
2.2.1 Piezoelectric effect
Piezoelectric effect is also known as either generator or sensor effect; the effect converts mechanical energy into electrical energy,
Priya, S. (2007).The mechanism of the piezoelectric effect is relatedly similar to the mechanism of electric dipole moments in solids. The piezoelectric effect can be found not only in monocrystalline materials but also in polycrystalline ferroelectric ceramics. In single crystal structure, the condition for the effect to occur is simply by formation of asymmetry in structure crystal lattice unit cell, which is generally a form below the Curie temperature Tc.
The decisive consequentiality for the piezoelectric effect is whenever a mechanical stress is applied to the piezoelectric material, the polarization P is changes Ok, K. M. et al., (2006). This phenomenon might either be caused by a re-configuration of the dipole-inducing or by re-orientation of molecular dipole moments resulting from the influence of the external stress.
2.2.2 Piezoelectric Coefficient
The piezoelectric coefficient is the parameter in piezoelectric a ceramic material that is aim to be controlled and altered to achieve certain value and controlling the piezoceramic properties suitable to application of the material. Some of the related piezoelectric coefficient are permittivity ε, piezo modulus dij, piezoelectric voltage
18.104.22.168 Permittivity ε
The permittivity, ε is the ratio of the absolute permittivity of the material by the permittivity in vacuum (ε0 = 8.85 × 10-12 F/m), as the absolute permittivity is a
quantification of the polarizability in the electrical field. The dependency of the dielectric displacement and the dielectric coefficient from the orientation of the electric field is designated by the corresponding indices, Yokoyama, S. et al.,(2006).
2.3 Electrical properties 2.3.1 Piezoelectric
Piezoelectric materials are utilized for fabrication of electrical devices that convert mechanical forces into electrical signals (direct piezo effect), inverse piezo effect where electrical signals is changes into mechanical forces, or electrical signals into electrical signals (utilization of both direct and inverse effects).
2.3.2 Piezoresistive effect
The piezoresistive effect is a transmutation in the electrical resistivity of a semiconductor when mechanical strain is present. Compare to the piezoelectric effect, the piezoresistive effect only affecting changes in electrical resistance.
rather than metal strain gauges, due semiconductor strain gauges that are much more sensitive to environmental surrounding, Mootanah, & Bader, (2006).
In silicon, the factors are two orders of magnitudes more sizeable voluminous than in metal. The resistance of n-conducting silicon mainly varies due to a shift of the three different conducting valley pairs, Sapmaz, et al., (2006). The shifting results to a spreading of the carriers between valleys with different mobility. This results in varying mobility dependent on the direction of current flow. The minor effect is due to the efficacious mass change cognate to transmuting shapes of the valleys. In p-conducting silicon the behaviour are more intricate and additionally result in mass changes and aperture transfer.
2.4 Piezoelectric Ceramic
Intrinsic piezoelectric ceramics have an unstructured polarization, Kong, & Wang, (2003) as the charge concentrations of the unit cells are discrete from each other. Plus, the axis of the lattice elongates in the direction of both the spontaneous strain occurs and polarization.The piezoelectric effect of natural monocrystalline materials Rochelle salt is relatively minuscule. However, for polycrystalline ferroelectric ceramics such as lead zirconate titanate (PZT) and barium titanate (BaTiO3) exhibit
more sizably voluminous displacements or induce more immensely colossal electric voltages.